A new ternary derivative of the Laves phases in the Mg-Co-Ga system.
Pavlyuk, Nazar; Dmytriv, Grygoriy; Pavlyuk, Volodymyr; Ciesielski, Wojciech; Rozdzynska-Kielbik, Beata; Indris, Sylvio; Ehrenberg, Helmut; Acta crystallographica Section B, Structural science, crystal engineering and materials 79 (2023) –; doi:10.1107/S2052520623004511

data_2312137
_publ_section_title
;
 A new ternary derivative of the Laves phases in the Mg-Co-Ga system.
;
_journal_coeditor_code           RA5132SUP1
_journal_issue                   4
_journal_name_full
'Acta crystallographica Section B, Structural science, crystal engineering and materials'
_journal_paper_doi               10.1107/S2052520623004511
_journal_volume                  79
_journal_year                    2023
_chemical_formula_moiety         'Co2 Ga2 Mg2'
_chemical_formula_sum            'Co Ga Mg'
_chemical_formula_weight         152.96
_space_group_crystal_system      hexagonal
_space_group_IT_number           194
_space_group_name_Hall           '-P 6c 2c'
_space_group_name_H-M_alt        'P 63/m m c'
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            4
_cell_length_a                   5.0151(5)
_cell_length_b                   5.0151(5)
_cell_length_c                   8.1086(9)
_cell_measurement_reflns_used    177
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      35.373
_cell_measurement_theta_min      4.693
_cell_volume                     176.62(3)
_computing_cell_refinement       'CrysAlis CCD (Oxford Diffraction, 2008)'
_computing_data_collection       'CrysAlis CCD (Oxford Diffraction, 2008)'
_computing_data_reduction        'CrysAlis RED (Oxford Diffraction, 2008)'
_computing_molecular_graphics    'DIAMOND (Brandenburg, 2006)'
_computing_publication_material  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXS-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.987
_diffrn_measured_fraction_theta_max 0.973
_diffrn_measurement_device_type  'Oxford Diffraction Xcalibur3 CCD'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0472
_diffrn_reflns_av_unetI/netI     0.0194
_diffrn_reflns_Laue_measured_fraction_full 0.987
_diffrn_reflns_Laue_measured_fraction_max 0.973
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            2830
_diffrn_reflns_point_group_measured_fraction_full 0.987
_diffrn_reflns_point_group_measured_fraction_max 0.973
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         35.373
_diffrn_reflns_theta_min         4.693
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    24.402
_exptl_absorpt_correction_T_max  0.783
_exptl_absorpt_correction_T_min  0.562
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details   '(CrysAlis RED; Oxford Diffraction, 2008)'
_exptl_crystal_colour            'metallic grey'
_exptl_crystal_density_diffrn    5.752
_exptl_crystal_density_meas      5.77(3)
_exptl_crystal_density_method    volumetric
_exptl_crystal_description       prism
_exptl_crystal_F_000             280.0
_exptl_crystal_size_max          0.030
_exptl_crystal_size_mid          0.020
_exptl_crystal_size_min          0.010
_refine_diff_density_max         0.917
_refine_diff_density_min         -0.923
_refine_diff_density_rms         0.225
_refine_ls_extinction_coef       0.018(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.274
_refine_ls_matrix_type           full
_refine_ls_number_parameters     14
_refine_ls_number_reflns         177
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.274
_refine_ls_R_factor_all          0.0264
_refine_ls_R_factor_gt           0.0254
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0289P)^2^+0.4871P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0642
_refine_ls_wR_factor_ref         0.0644
_reflns_Friedel_coverage         0.000
_reflns_number_gt                172
_reflns_number_total             177
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            ra5132sup1.cif
_cod_data_source_block           I-MgCoGa
_cod_original_cell_volume        176.62(4)
_cod_database_code               2312137
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              69122
_shelx_hkl_checksum              67932
_cod_database_fobs_code 2312137